Norma ASTM para la realizacion de reometrias con un reómetro de disco oscilante...
Designation: D 2084 – 01
Standard Test Method for
Rubber Property—Vulcanization Using Oscillating Disk Cure Meter1 This standard is issued under the ﬁxed designation D 2084; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript superscript epsilon epsilon (e) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense.
1. Scope Scope
1.1 This test method describes describes the use of the oscillating oscillating disk cure meter for determining selected vulcanization characteristics of vulcanizable rubber compounds. 1.2 The values values stated in SI units are to be regarded regarded as the standard. The values given in parentheses are for information only. 1.3 ISO 3417 is very similar to to this test method. It has minor minor technical differences that are not considered to be signiﬁcant. standard d does does not purpor purportt to addre address ss all of the 1.4 This standar safet safetyy conc concer erns ns,, if any any, asso associ ciate ated d with with its use. use. It is the the responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use.
3.1 Deﬁnitions of Terms Speciﬁc to This Standard: 3.1.1 The following following measurements measurements may be taken from the curve of torque versus time (see Fig. 1). cure rate rate index index—measu 3.1.2 cure —measure re of rate rate of vulcan vulcaniza izatio tion n based on the difference between optimum vulcanization and incipient scorch time. maximum, m, platea plateau, u, or highes highestt torque torque—measure 3.1.3 maximu —measure of stiffness or shear modulus of the fully vulcanized test specimen at the vulcanization temperature. 3.1.4 minimum —measu sure re of the the stif stiffn fnes esss of the the minimum torque torque—mea unvulcanized test specimen taken at the lowest point of the curve. 3.1.5 time to incipient cure (scorch time)—measure of the time at which vulcanization begins. 3.1.6 time to a percentage of full cure—measure —measure of optimum cure based on the time to develop some percentage of the highest torque or difference in torque from the minimum. 3.1.7 torque— for an oscillating shear cure meter , the value measured by a torque transducer at the peak strain amplitude of the oscillating cycle.
2. Referenced Documents 2.1 ASTM Standards: D 1349 Practice Practice for Rubber—St Rubber—Standar andard d Temperature emperaturess for 2 Testing D 3185 3185 Test Method Methodss for Rubber Rubber—Ev —Evalu aluati ation on of SBR (Styrene-Butadiene Rubber) Including Mixtures With Oil 2 D 3186 3186 Test Method Methodss for Rubber Rubber—Ev —Evalu aluati ation on of SBR (Styrene-Butadiene Rubber) Mixed With Carbon Black or Carbon Black and Oil 2 D 3187 3187 Test Method Methodss for Rubber Rubber—Ev —Evalu aluati ation on of NBR 2 (Acrylonitrile-Butadiene Rubber) D 3190 3190 Test Methods Methods for Rubber—Eva Rubber—Evaluati luation on of ChloroChloro2 prene Rubber (CR) D 4483 Practice for Determining Determining Precision for Test Test Method Standards in the Rubber and Carbon Black Industries 2 Standard: 2.2 ISO Standard: ISO 3417 Rubber—Measurement Rubber—Measurement of Vulcanization Vulcanization Characteristics With the Oscillating Disk Rheometer 3
4. Summary Summary of Test Method 4.1 A test test specim specimen en of vulcan vulcaniza izable ble rubber rubber compou compound nd is insert inserted ed into into the cure cure meter meter test test cavity cavity and after after a closur closuree action is contained in a sealed cavity under positive pressure. The cavity cavity is mainta maintaine ined d at some some elevat elevated ed vulcan vulcaniza izatio tion n temperature. The rubber totally surrounds a biconical disk after the dies are closed (see Fig. 2). The disk is oscillated through a small rotational amplitude (1° or 3°) and this action exerts a shear strain on the test specimen. The force required to oscillate or rotate rotate the disk disk to maxim maximum um amplit amplitude ude is contin continuou uously sly recorded as a function of time, with the force being proportional to the shear modulus (stiffness) of the test specimen at the test temperature. This stiffness ﬁrst decreases as it warms up; then it increases due to vulcanization. The test is completed when when the record recorded ed torque torque either either rises rises to an equili equilibri brium um or maximum value, or when a predetermined time has elapsed. The time required to obtain a cure curve is a function of the
1 This test method is under the jurisdiction of ASTM Committee D11 on Rubber and is the direct responsibility responsibility of Subcommittee Subcommittee D11.12 D11.12 on Processability Processability Tests. Current Current edition approved approved Aug. 10, 2001. Published Published October 2001. 2001. Originally Originally published as D 2084 – 71 T, replacing Methods D 2705 and D 2706. Last previous edition D 2084 – 95. 2 Annual Book of ASTM Standards Standards,, Vol 09.01. 3 Available Available from American National Standards Institute, 25 W. 43rd St., 4th Floor, New York, NY 10036.
Copyright © ASTM, 100 Barr Harbor Drive, West Conshohocken, PA 19428-2959, United States.
Left Curve: Cure to Equilibrium Torque. Middle Curve: Cure to a Maximum Torque with Reversion. Right Curve: Cure to No Equilibrium in Maximum Torque.
FIG. 1 Types of Cure Curve
FIG. 2 Cure Meter Assembly
characteristics of the rubber compound and of the test temperature (see Fig. 1 for typical cure curves).
dies is shown in Fig. 3 and Fig. 4 with dimensions and tolerances (see Table 1). The top and bottom surfaces of the die cavity shall contain rectangularly shaped grooves arranged radially about the center and spaced at 20° intervals. Each die shall have a well or hole drilled from the side to accommodate a temperature sensor inserted through the platen. The lower dies shall have a hole in the center to allow for the insertion of the disk shaft. A suitable low-friction seal shall be provided in this hole to prevent material leaking from the cavity. 6.2.3 Disk —The biconical disk (see Fig. 5) shall be fabricated from tool steel having a minimum Rockwell Hardness of HRC 50. The disk shall be ﬁtted with a stem that ﬁts into the torque shaft. The disk is shown in Fig. 5 (see Table 2). 22.214.171.124 Disk wear will affect test results. A disk worn to such an extent that the disk diameter is less than the minimum diameter shown in this procedure shall not be used. 126.96.36.199 The standard frequency of the rotary oscillation of the disk shall be constant at 1.7 Hz (100 cpm). Other frequencies may be used, if required. 188.8.131.52 A rotary drive system shall be provided for oscillatory rotation of the disk. The amplitude of oscillation of the unloaded disk shall be constant at 6 1.00° with a tolerance of 60.03° about the center position, that is, a total amplitude of 2°. Other amplitudes may be used, if speciﬁed.
5. Signiﬁcance and Use 5.1 This test method is used to determine the vulcanization characteristics of (vulcanizable) rubber compounds. 5.2 This test method may be used for quality control in rubber manufacturing processes, for research and development testing of raw-rubber compounded in an evaluation formulation, and for evaluating various raw materials used in preparing (vulcanizable) rubber compounds. 6. Apparatus 6.1 Cure meter , consists of the following major components: specimen chamber and closure mechanism, temperature control system, rotor drive and torque measuring system (see Fig. 2 for a detailed drawing of cure meter assembly). 6.2 Specimen Chamber —Consists of platens, dies, and a biconical disk. 6.2.1 Platens—Two platens made of aluminum alloy, each containing an electric heater, and each having in the center, a cavity to accommodate a die and from the side, a well for inserting a temperature sensor. 6.2.2 Dies—Two which form a cavity when closed and which shall be fabricated from tool steel having a minimum Rockwell Hardness HRC 50. The geometry of the standard
NOTE 1—Where the effect of surface contamination on the disk is not
FIG. 3 Lower Die a problem, greater sensitivity in determining curing characteristics may be obtained using 6 3° angle of oscillation.
6.2.4 Die Closing Mechanism—A pneumatic cylinder or other device shall close the dies and hold them closed during the test with a force of 11.0 6 0.5 kN (2500 6 100 lbf).
FIG. 4 Upper Die TABLE 1 Die Dimensions
NOTE 2—The manufacturer recommends the source air pressure be adjusted to 345 kPa (50 psi). Provisions are made for this adjustment in the instrument. Therefore, 345 kPa acting on the instrument’s 203-mm (8-in.) diameter air cylinder will produce a force of 11 kN (2500 lbf) on the die per the following equation: F 5 P
S D p D2 4
Code A B C D E F G H I J K L M N O P Q R
where: F = closure force on die, = source air pressure, and P D = diameter of piston in pneumatic cylinder. To calculate maximum cavity pressure, the effect of this force acting on the surface area of the upper die may be calculated per the following equation: Pc 5
where: Pc = pressure on sample in upper die cavity, and d = diameter of upper die cavity (55.9 mm (2.2 in.)).
~For example, P c 5 5
60.13 60.25 60.13 60.13 60.13 60.1 60.13 60.06 60.40 60.40 60.05 60.03 60.01 60.03 60.13 60.03 60.05 60.03
55.88 10.64 7.94 18.26 1.57 0.8 4.76 24.07 12.70 2.38 54.61 41.91 5.35 1.65 4.57 15.38 5.08 41.91
10 000 12.06
5 829 psi.
6.3 Temperature Controlling System—A temperature controller shall be provided for maintaining the dies within 60.5°C (61°F) of the speciﬁed test temperature.
~3.14!~2.2!2 10 000 5 ~3.14!~4.84!
D 2084 use of any suitable data collection device, including printers, plotters, and computers. NOTE 4—Direct proportionality between torque and stiffness cannot be expected under all test conditions, particularly in higher torque ranges, because elastic deformation of the disk shaft and driving device must be taken into account. However, for routine quality control test purposes corrections are not necessary.
7. Sampling 7.1 The sample shall be taken from a vulcanizable rubber compound as required by the mixing method or other sampling instructions. 7.2 The sample shall be in sheeted form, at room temperature, and as free of air as possible. 8. Test Specimen 8.1 A circular test specimen taken from a sample shall be 30 6 2 mm (1.2 6 0.1 in.) in diameter and 11.5 6 1.5 mm (0.45 6 0.05 in.) in thickness or equivalent to a volume of 9 cm 3 (0.5 in.3). 8.2 The test specimen is considered to be of proper size when a small bead of compound is extruded uniformly around the periphery of the die as it is closed. This is achieved when the specimen volume is between 8 and 11 cm 3(9 to 13 g of rubber compound with a speciﬁc gravity of 1.15). Undersized specimens can cause low cavity pressure and low torque readings. Oversized specimens cool the dies excessively during the early part of the test cycle affecting the vulcanization characteristics. 9. Test Temperatures FIG. 5 Biconical Disk
9.1 The standard test temperature shall be 160°C (320°F). 9.2 The test temperature tolerance shall be 60.5°C (61.0°F). 9.3 Tests may be carried out at other temperatures, if required. They should be selected in accordance with Practice D 1349.
TABLE 2 Disk Dimensions Code S T U VA
Groove width Groove depth Groove lengths, min
Groove width Groove depth Groove lengths, min
35.55 0.80 6.28° 0.80 0.8 7.5 12.5 0.80 0.8 7.5 9.5 9.50
60.01 60.03 60.08° 60.05 60.1
10. Calibration 10.1 The cure meter shall be calibrated mechanically in accordance with the manufacturer’s instructions. 10.2 Provisions shall be made for electronic veriﬁcation of the recorder and for torque transducer calibration by means of a resistor incorporated in the torque measuring circuit that simulates an applied torque of speciﬁed value. 10.3 The cure meter shall be calibrated with the torque standard supplied by the manufacturer any time the results are suspected of being inaccurate, after any repairs, any change in arc, or frequently enough to ensure the maintenance of proper calibration. The cure meter shall read zero when running empty and read the certiﬁed value with the torque standard inserted.
Grooves on top and bottom surfaces should be displaced 5°.
6.4 Torque Measuring System—The torque measuring system shall consist of a device, such as a torque transducer, producing a signal that is directly proportional to the torque required to oscillate the disk. A recorder to record the maximum amplitude signal from the torque transducer shall be provided. The recorder shall have a full-scale deﬂection response on the torque scale of 1 s or less and be capable of recording the torque with accuracy of 60.5 % of the torque range. Four torque ranges shall be provided; 0 to 25, 0 to 50, 0 to 100, and 0 to 200 dN·m (or 0 to 25, 0 to 50, 0 to 100, and 0 to 200 lbf· in.)
11. Procedure 11.1 Preparation for Test : 11.1.1 Bring the temperature of both dies to the temperature of test with the disk in place and the dies in the closed position. Set recorder range to zero and adjust the recorder pen to zero torque and zero time position on the chart. Select the correct running time and choose the torque range to give maximum torque in the upper half of the recorder chart.
NOTE 3—The term “recorder” as used in this test method implies the
D 2084 11.1.2 “Running Zero” may be checked at this point and should be off no more than 0.5 dN·m (or 0.5 lbf·in.). If in excess of this, check the cure meter for frictional drag that could be caused either by bad bearings, by improper friction seal (6.2.2), by rotor misalignment, or by sample “build-up” around the rotor shaft. If the error persists, consult the manufacturers manual. 11.2 Loading the Cure Meter : 11.2.1 Open the dies, place the test specimen (Note 5 and Note 6) on top of the disk and close the dies. This operation must be completed within 20 s. 11.2.2 Start the recorder at the instant the dies are closed. The disk may be oscillating at zero time or oscillation may be started not later than 1 min after the dies are closed. In the latter case, report preheat as required in 12.1.8.
184.108.40.206 t S1 is equal to the time to 1 dN·m (or lbf·in.) rise above M L; is used with 1° amplitude. 220.127.116.11 t S2 is equal to the time to 2 dN·m (or 2 lbf·in.) rise above M L; is used with 3° (and 5°) amplitudes. 12.2.4 Cure time, min. 18.104.22.168 t x is equal to the time to x % of torque increase or t x = minutes to M L + x( M H − M L)/100 torque.
NOTE 5—When testing sticky rubber compounds, cellophane, or other thin ﬁlm that will not melt at the test temperature, may be inserted below and above the test specimen, but not against the rotor. This prevents the rubber from sticking to the dies. Suitable ﬁlm materials are Dupont 600 PD/001,4 Avisco 300P1,5 or Polyester Film Mylar Type A-100.6 NOTE 6—A deposit of material from the rubber compounds under test may build up on the disk and dies. This may affect the ﬁnal torque values. It is suggested that stable vulcanizable rubber compound be tested daily to detect this occurrence. If such contamination develops, it may be removed by cleaning with a noncorrosive compound or solution that does not degrade the aluminum insert contained in the upper die of most cure meters. After solvent cleaning one or two runs on a nonessential rubber compound are required to eliminate solvent or residue completely. Abrasive cleaning may be used with caution. The recommended cleaner is 220 grit aluminum oxide.
13. Precision and Bias
NOTE 7—This test method of determining the cure times is considered the standard test method.
22.214.171.124 t x is equal to the time to x % of maximum torque, or t x = minutes to x M H /100 torque. NOTE 8—This is an alternative test method for cure time determination. The most commonly used values of x are 50 and 90.
12.2.5 Cure Rate Index = 100/(cure time − scorch time). 13.1 This precision and bias section has been prepared in accordance with Practice D 4483. Refer to Practice D 4483 for terminology and other statistical calculation details. 13.2 All precision data were obtained using the diaphragm upper die shown in Fig. 4. The use of the alternative solid die shown in Fig. A1.1 may cause different results. 13.3 Both Type 1 and Type 2 precision results are given in Table 3. For both types of precision repeatability and reproducibility are short term; a period of a few days separates replicate test results. A test result is the test value, as speciﬁed by this test method, obtained on one determination or measurement of the property or parameter in question. 13.4 For the Type 1 precision, four compounds (or materials) were used; these were tested in eleven laboratories on two different days (see Table 3). 13.5 For the Type 2 precision, the precision results reported in Table 3 represent pooled average values obtained from four (other) rubber evaluation standards; Test Methods D 3185 (SBR, OE-SBR) and Methods D 3186 (SBR-BMB), D3187 (NBR), and D3190 (CR). These precision values are derived from interlaboratory programs with two different types of materials (for each rubber as listed above), in seven laboratories with the mixing and testing both conducted on two different days essentially one week apart. 13.6 The precision of this test method may be expressed in the format of the following statements that use what is called an “appropriate value” of r , R, (r ) , or ( R), that is, that value obtained from Table 3, to be used in decisions about test results (obtained with the test method). 13.7 Repeatability—The repeatability, r , of this test method has been established as the appropriate value for any parameter as tabulated in Table 3. Two single test results, obtained under normal test method procedures, that differ by more than this tabulated r must be considered as derived from different or nonidentical sample populations. 13.8 Reproducibility—The reproducibility, R, of this test method has been established as the appropriate value for any parameter as tabulated in Table 3. Two single test results obtained in two different laboratories, under normal test method procedures, that differ by more than the tabulated R must be considered to have come from different or nonidentical sample populations.
12. Report 12.1 Report the following information on the sample and instrument used: 12.1.1 Sample or specimen identiﬁcation, or both, 12.1.2 Method of specimen preparation (for example, amount of milling), 12.1.3 Make and model of the cure meter, 12.1.4 Temperature of the dies, 12.1.5 Amplitude of oscillation used, reported as half of total amplitude, 12.1.6 Frequency of oscillation, Hz (or cpm), 12.1.7 Recorder range, 12.1.8 Full-scale recorder time, and 12.1.9 Preheat time, if not zero. 12.2 Test results reported are normally chosen from the following parameters (refer to Fig. 1 for guidance). The conversion from dN·m to lbf·in. is: 1.13 (dN·m) = 1.00 (lbf·in.). 12.2.1 M L—Minimum torque, dN·m (lbf·in.). 12.2.2 Maximum torque—All in dN·m (or lbf·in.). 126.96.36.199 M HF—Maximum torque where curve plateaus. 188.8.131.52 M HR—Maximum torque of reverting curve. 184.108.40.206 M H—Highest torque attained during speciﬁed period of time when no plateau or maximum torque is obtained. 12.2.3 Scorch time, min.
Dupont 600 PD/001 is suitable for this purpose. Avisco 300P1 is suitable for this purpose. 6 Polyester Film Mylar Type A-100 is suitable for this purpose. 5
D 2084 TABLE 3 Precision NOTE 1—S r = within laboratory standard deviation. r = repeatability (in measurement units). (r ) = repeatability (in percent). S r = between laboratory standard deviation. R = reproducibility (in measurement units). ( R) = reproducibility (in percent). Test Parameter Type 1 Precision: M L(dN·m) M H(dN·m) t sl (min) t 50 (min) t 90 (min) Type 2 Precision: M L(dN·m) M H(dN·m) t sl (min) t 50 (min) t 90 (min) 8 8
Range of Values
Between Laboratory (r )
7.1 28.4 2.3 3.9 6.4
to to to to to
9.7 38.9 5.3 8.8 14.0
8.4 33.7 3.8 6.4 10.2
0.158 0.181 0.12 0.15 0.20
0.45 0.51 0.34 0.43 0.57
5.4 1.5 9.0 6.7 5.6
1.36 1.98 0.25 0.34 0.60
3.85 5.60 0.71 0.96 1.70
45.8 16.6 18.7 15.0 16.7
7.6 32.0 4.4 7.7 15.9
to to to to to
9.8 47.7 5.8 9.9 18.0
8.7 39.9 5.1 8.8 17.0
0.215 0.35 0.12 0.18 0.19
0.61 0.99 0.34 0.51 0.54
7.0 2.5 6.7 5.8 3.2
0.735 2.60 0.37 0.90 1.50
2.08 7.36 1.05 2.55 4.25
23.9 18.4 20.6 29.0 25.0
These are estimated values, using the mid-point of the range for the parameter mean value. Type 1 precision is obtained from fully prepared test specimens (compounds mixed in one laboratory); these are circulated to all participating laboratories. Type 2 precision is obtained by circulating all compounding materials (drawn from a common source) to each participating laboratory. The mixing to prepare the compound is done in each laboratory and therefore mixing variation is part of the “total test” variation or test precision.
13.9 Repeatability and reproducibility expressed as a percentage of the mean level, ( r ) and ( R), have equivalent application statements as 13.7 and 13.8 for r and R . For the ( r ) and ( R) statements, the difference in the two single test results is expressed as a percentage of the arithmetic mean of the two test results. 13.10 Precision (International Interlaboratory Testing)— The Appendix gives precision results obtained in an international interlaboratory program conducted in ISO Technical Committee 45 on Rubber/Rubber Products in 1984/1985. These results are given for additional background on a broadbased comprehensive interlaboratory program. Please refer to
the appendix for details and a full report on the precision results. 13.11 Bias—In test method terminology, bias is the difference between an average test value and the reference (or true) test property value. Reference values do not exist for this test method since the value (of the test property) is exclusively deﬁned by the test method. Bias, therefore, cannot be determined. 14. Keywords 14.1 compounds; ODR oscillating disk cure meter; vulcanization characteristics
ANNEX (Mandatory Information) A1. ALTERNATIVE UPPER DIE
A1.1 This annex describes an alternative upper die for use in the oscillating disk cure meter (ODC). This die does not contain a diaphram as shown in the die in Fig. 4.
and then to maintain essentially constant pressure on the specimen as it shrinks slightly in volume during vulcanization.
A1.2 Some manufacturers of ODC instruments furnish upper dies with a diaphram while others do not.
A1.4 The precision and bias observed with the alternative solid upper die as well as any differences in observed results have not been determined.
A1.3 The stated purpose of the diaphram die is to allow the diaphram to be ﬂexed when the dies are closed on a specimen
A1.5 The solid upper die is shown in Fig. A1.1. Dimensions are listed in Table 1.
FIG. A1.1 Alternative Upper Die
APPENDIXES (Nonmandatory Information) X1. INTERNATIONAL INTERLABORATORY TESTING TABLE X1.1 Compound Formulations (ISO 3417-ITP)
X1.1 This appendix gives the precision results of an international interlaboratory Oscillating Disc Cure Meter (ODC) test program conducted in ISO TC-45 in 1984 and 1985. It is added as an appendix to this test method to give additional information on the precision of ODC testing. The ISO/TC45 standard that is analogous to Test Method D 2084 is ISO 3417.
Material SBR 1502 SBR 1712 A BR (CB441) B Zinc oxide Stearic acid IRB Number 5C N330 Process OilD DPPD E AntiozonantF TBBS G TMTDH Sulfur
X1.2 The practice for analysis and expression of precision results for ISO TC45 is equivalent in its basic fundamentals and format to Practice D 4483. X1.3 Test Details: X1.3.1 An interlaboratory test program (ITP) was organized in late 1984 to obtain precision results. Four compounds with a range of cure properties were mixed and prepared in one laboratory, sealed in metal foil packets, and distributed to laboratories located in 19 countries in Europe, Asia, and North and South America. Tests were conducted in late January and early February 1985 according to the following schedule: X220.127.116.11 Part I of 160C —One test (determination) on each of two days, one week apart, for all four compounds. X18.104.22.168 Part II of 150C —One test on each of two days, one week apart, for all four compounds. X1.3.2 The formulations for the four compounds are listed in Table X1.1. Compound A has a moderate black level with a non-free sulfur (TMTD) cure system. Compounds B and C are relatively high black with conventional cure systems. Com-
Formulations Used A
100.0 ... ... 5.0 1.0 ... 45.0 ... ... ... ... 3.0 ... __ 1.13
... 68.8 68.8 5.0 1.5 80.0 ... 8.8 1.5 1.5 1.2 ... 2.0 __ 1.16
... 137.5 ... 5.0 1.5 60.0 ... 5.0 1.5 1.5 1.0 ... 2.0 __ 1.16
100.0 ... ... 5.0 1.5 ... ... 5.0 1.5 1.5 1.0 ... 2.0 __ 0.98
37.5 (phr) oil extended SBR. 37.5 (phr) oil extended, BR rubber. C ASTM Committee D-24 Industry Reference Carbon Black Number 5. D Sundex 7260T or equivalent. E Dimethyl-butylphenyl-phenylene diamine. F Trimethyl-dihydroquinoline. G N-tert-butyl-2-benzothiazole-sulfenamide. H Tetramethylthiuram disulﬁde. B
pound D is a gum compound with a conventional cure system. X1.3.3 A Type 1 precision was measured in the ITP (no processing operations required on the circulated materials in any given laboratory). The time period for repeatability and reproducibility is on a scale of days. X1.3.4 A test result is (the test value) obtained from one 7
D 2084 measurement or determination with the ODC at any temperature. X1.3.5 A total of 50 laboratories participated in Part I, and 45 laboratories participated in Part II in addition to their participation in Part I.
results for the temperature nearest to the actual test temperature under consideration. X22.214.171.124 Enter the Summary Precision Result section of either Table X1.2 or X1.3 at an average material value nearest to the test data average under consideration. This will give the applicable r , (r ), R, and ( R) for use in the decision process. X126.96.36.199 With these r and (r ) values the following general repeatability statements may be used to make decisions. For an absolute difference, the difference, | x1 − x 2 |, between two measured ODC parameters values, found on (presumed) identical material samples under normal and correct ODC operation conditions, will exceed the tabulated r , on average not more than once in 20 cases. For a percentage difference, the percent difference, | x1 − x 2 | /( x1 + x 2)/2]100, between two measured ODC parameter values, found on (presumed) identical material samples under normal and correct ODC operation conditions, will exceed the tabulated ( r ), on average not more than once in 20 cases.
X1.4 Precision Results: X1.4.1 The precision results for both Parts I and II are given for ﬁve ODC cure parameters. These ﬁve parameters are as follows: X188.8.131.52 M L—Minimum torque (N·m). X184.108.40.206 M HF—Maximum torque (N·m). X220.127.116.11 t s—Scorch time, (minutes). X18.104.22.168 t 1c (50)—50 % cure time, (minutes). X22.214.171.124 t 1c (90)—90 % cure time, (minutes). X1.4.2 For Part I of 160C, the precision results are given in Table X1.2. X1.4.3 For Part II of 150C, the precision results are given in Table X1.3.
X126.96.36.199 With these R and ( R) values the following general reproducibility statements may be used to make decisions. For an absolute difference, the difference | x1 − x 2 |, between two independently measured ODC parameter values, found in two laboratories using normal and correct ODC procedures on identical test material samples, will exceed the tabulated reproducibility R, not more than once in 20 cases. For a percentage difference, the percent difference, | x1 − x 2 | /( x1 + x 2)/2]100, between two independently measured ODC parameter values, found in two laboratories using normal and
X1.5 Use of Precision Results: X1.5.1 The general procedure for using precision results is with the symbol | x1 − x 2 | designating a positive difference, that is, without regard to sign. The symbol x refers to any parameter value. X188.8.131.52 Select the ODC parameter on which decisions are to be made. Find in Table X1.2 (160C) or Table X1.3 (150C) the Summary section for this parameter. If the tests and data under consideration are not at 150 or 160C, select the summary
TABLE X1.2 ISO 3417: Type 1—Precision of 160 °C Parameter 1—Min torque, ML (N-M) 160 °C Final Summary Table: Precision Values Averages given in increasing order Material 4. Compound D 3. Compound C 2. Compound B 1. Compound A Pooled values
Average 0.39 0.70 0.99 1.65 0.92
0.0315 0.0316 0.0339 0.0656 0.0432
0.0892 0.0893 0.0960 0.1857 0.1223
23.040 12.700 9.652 11.249 13.298
0.1404 0.1997 0.4399 0.1442 0.2645
0.3973 0.5652 1.2448 0.4081 0.7486
102.649 80.380 125.147 24.715 81.422
Parameter 2—Max torque, MHF (N-M) 160 °C Final Summary Table: Precision Values Averages given in increasing order Material 4. Compound D 3. Compound C 2. Compound B 1. Compound A Pooled Values
Average 2.21 2.71 3.26 4.26 3.11
0.0582 0.0511 0.0750 0.0546 0.0605
0.1646 0.1446 0.2123 0.1544 0.1713
7.447 5.328 6.521 3.621 5.506
0.1996 0.2207 0.2625 0.3628 0.2686
0.5648 0.6246 0.7430 1.0266 0.7602
25.550 23.007 22.820 24.073 24.432
Parameter 3—Scorch time, (min) 160 °C Final Summary Table: Precision Values Averages given in increasing order Material 1. Compound A 4. Compound D 2. Compound B 3. Compound C Pooled Values
Average 1.41 5.04 5.08 5.57 4.32
0.1028 0.2017 0.1836 0.2302 0.1854
0.2910 0.5708 0.5197 0.6515 0.5247
20.580 11.324 10.222 11.689 12.140
0.1547 0.7011 0.7278 0.6752 0.6234
0.4377 1.9842 2.0598 1.9109 1.7642
30.957 39.364 40.512 34.284 40.822
D 2084 TABLE X1.3 ISO 3417: Type 1—Precision of 150 °C NOTE 1—Sr = repeatability standard deviation. r = repeatability = 2.83 (square root of the repeatability variance). (r ) = repeatability (as percentage of material average). SR = reproducibility standard deviation. R = reproducibility = 2.83 (square root of the reproducibility variance). R ( ) = reproducibility (as percentage of material average). Parameter 1—Min torque, ML (N-M) 150 °C Final Summary Table: Precision Values Averages given in increasing order Material 4. Compound D 3. Compound C 2. Compound B 1. Compound A Pooled Values
Average 0.40 0.69 0.77 1.74 0.90
0.0300 0.0403 0.0258 0.0517 0.0384
0.0848 0.1141 0.0730 0.1463 0.1086
21.000 16.448 9.511 8.399 12.098
0.1286 0.1025 0.0743 0.1616 0.1221
0.3639 0.2901 0.2101 0.4574 0.3457
90.135 41.798 27.376 26.250 38.505
Parameter 2—Max torque, MHF (N-M) 150 °C Final Summary Table: Precision Values Averages given in increasing order Material 4. Compound D 3. Compound C 2. Compound B 1. Compound A Pooled Values
Average 2.31 2.82 3.39 4.34 3.20
0.0324 0.0684 0.0642 0.0787 0.0633
0.0916 0.1937 0.1818 0.2228 0.1793
3.960 6.861 5.354 5.134 5.594
0.1942 0.2431 0.2654 0.2464 0.2397
0.5495 0.6878 0.7511 0.6972 0.6783
23.768 24.364 22.124 16.066 21.169
Parameter 3—Scorch time, (min) 150 °C Final Summary Table: Precision Values Averages given in increasing order Material 1. Compound A 2. Compound B 4. Compound D 3. Compound C Pooled Values
Average 1.99 8.61 8.77 9.73 7.31
0.1141 0.4932 0.2524 0.3233 0.3266
0.3230 1.3958 0.7143 0.9150 0.9243
16.265 16.213 8.149 9.406 12.650
0.2471 1.2572 0.6697 1.3838 0.9867
0.6992 3.5577 1.8951 3.9161 2.7924
35.214 41.325 21.621 40.257 38.217
Parameter 4—50 % cure time, (min) 150 °C Final Summary Table: Precision Values Averages given in increasing order Material 1. Compound A 2. Compound B 3. Compound C 4. Compound D Pooled Values
Average 5.56 13.34 17.20 17.56 13.46
0.2100 0.5602 0.3975 0.3393 0.3983
0.5943 1.5852 1.1250 0.9603 1.1272
10.691 11.882 6.539 5.470 8.374
0.4654 0.9905 1.1619 1.1049 0.9726
1.3172 2.8032 3.2883 3.1269 2.7525
23.696 21.011 19.113 17.812 20.448
Parameter 5—90 % cure time, (min) 150 °C Final Summary Table: Precision Values Averages given in increasing order Material 1. Compound A 2. Compound B 3. Compound C 4. Compound D Pooled Values
Average 11.91 19.90 30.07 33.52 23.91
0.6954 0.7055 0.6387 0.9787 0.7671
1.9680 1.9964 1.8075 2.7699 2.1708
16.521 10.031 6.010 8.264 9.080
1.2683 1.4111 2.1003 2.5473 1.9092
3.5894 3.9934 5.9439 7.2088 5.4030
30.133 20.065 19.763 21.507 22.599
correct ODC procedures on identical material samples, will exceed the tabulated reproducibility ( R), not more than once in 20 cases.
D 2084 X2. HISTORY OF THE OSCILLATING DISK CURE METER
X2.1 Oscillating disk cure meters were ﬁrst made commercially available in 1963. The ﬁrst units oscillated at a frequency of three cycles per minute, typically at 63° of arc. The dies (SCD) for these early cure meters were commonly a 2-in. square cavity 0.4 in. high, with a biconical rotor centered in the cavity. A typical rubber sample of 1.15 speciﬁc gravity weighed 22 g, and was loaded in two pieces, above and below the rotor. A20 to 60-s preheat was required after closure before collecting data. The strain on the sample at 3° arc was 21 %.
dies and rotor. Higher strain leads to higher torques, and the smaller specimen (10 to 12 g for a stock with a speciﬁc gravity of 1.15) gives a cure curve with a signiﬁcantly different shape, as shown in Fig. X2.2. Higher torques have been shown to cause slippage at the surface of the rotor for many stocks, and that slippage is a potential source of variation in test results. Studies conducted with the smaller dies and rotor indicated slippage due to rotor contamination was common above 50 in.·lbs of torque. As a result, Test Method D 2084 speciﬁes a 1° arc of oscillation as standard, with a 16 % shear strain.
X2.2 Frequencies of oscillation of 10, 100, and 900 cpm were made available over the next ﬁve years. These created different curve shapes due to the heat energy added to the cavity in working the rubber, breakdown of polymer structure when curing under dynamic conditions, and the shear rate dependence of the rubber ﬂow resistance. Fig. X2.1 compares the cure meter curves for the various speeds of oscillation using the square dies and an arc of 6 3°.
X2.5 The curves obtained with MPC dies at 1° arc were used as standards until 1987, when further reductions in the temperature recovery time became possible due to improved temperature controllers. X2.6 Another improvement introduced at this time was the reduction of the mechanical compliance of the rotor drive system for improved reproducibility between instruments. The improved mechanical design increased maximum torques, but lowered minimum torques by reducing friction. Faster temperature recovery has two advantages: ﬁrst, the cure is closer to the desired cure temperature of the test for more accurate results; second, the potential for variation in results due to cooling of the rotor during loading and unloading is greatly reduced. Table X2.1 illustrates the potential operator effects.
X2.3 When the oscillating disk cure meter was ﬁrst proposed as an ASTM standard in 1968, a smaller, productionsized table model of the cure meter was introduced along with a new die that was 2 in. in diameter (LPC dies). This circular die had the same height and used the same rotor as the square dies. The LPC die produced similar torque values for minimum and maximum torques as the SCD die. The sample could be loaded as one piece on top of the rotor for most stocks. The practice of adding a preheat, as commonly used with the SCD die, was eliminated. The elimination of the preheat time led to slightly faster cures for the LPC die. Another advantage of this die was the ﬂat lower die surface which allowed easier removal of the cured sample for most stocks.
X2.7 As part of the continuing evolution in cure meter design, a number of manufacturers have introduced rotorless cure meters. These cure meters use a sample of 3 to 5 g, with a thinner cross section to obtain more rapid temperature recovery and more uniform temperature throughout the specimen. The dies are usually directly heated, and smaller in mass than for the oscillating disk cure meters, so that faster temperature recovery can be achieved. By eliminating the rotor, the surface area under load is reduced so that smaller torque values are achieved. Faster temperature recovery leads to faster cure times. Fig. X2.3 compares typical cure curves for an SBR stock from the rotorless and oscillating disk cure meters.
X2.4 In 1971, a smaller version of the LPC die, called the MPC die, was adopted in conformance with Test Method D 2084. The MPC die used a rotor with a different conical angle. At 3° of arc, the strain is 48 % versus 21 % for the larger
FIG. X2.1 Comparison of Oscillation Frequencies Using the Square Die and 6 3°Arc
FIG. X2.2 Comparison of Cure Meter Dies
D 2084 TABLE X2.1 Operator Effects on ODR Cure Meter Tests Sample Loading Variable Slow Temperature Recovery: Optimum loading time (20 s) 2-min loading time % change with loading time Rapid Temperature Recovery: Optimum loading time (20 s) 2-min loading time % change with loading time
Cure Times, min TS2
2.01 2.33 15.9
3.51 3.90 11.1
5.86 6.33 8.0
1.71 1.86 8.8
3.06 3.23 5.6
5.40 5.60 3.7
FIG. X2.3 Comparison of Cure Meters Using SBR Stock
X3. ALTERNATIVE BICONICAL DISK
X3.1 This appendix describes an alternative biconical disk for use in the oscillating disk cure meter (ODC). The alternative disk described in this appendix is directly heated for the purpose of maintaining the temperature of the disk at the speciﬁed test temperature during the total testing interval.
biconical disk show in Fig. 5. This modiﬁcation has provisions for directly controlling the disk temperature, as shown in Fig. X3.2. In this example, an electrical heater and temerature sensor are located in a metal tube, which is inserted in the disk throught a vertical well in the disk shaft. The well is typically 33 cm (0.130 in.) in diameter and extends to within 0.25 cm (0.100 in.) of the disk apex. The insertion tube diameter is typically 0.1 cm (0.005 in.) less than the well diameter, allowing easy tube removal for cleaning.
X3.2 Some manufactures of ODC instruments offer a heated rotor, while others do not. If the disk is heatd, both torque values and cure times may be signifcantly altered. Fig. X3.1 shows an example of the difference in cure curves. Test results between ODC tests using heated and unheated disks canot be compared without taking the differences in heating into account. When a heated rotor is used, it shall be reported with the test results.
X3.4 A temperature controller shall be provided for maintaining the disk temperature within 6 0.5°C (6 1.0°F) of the speciﬁed test temperature.
X3.3 The alternative heated disk is a modiﬁcation of the
FIG. X3.1 Comparison of Cure Curves With Heated and Unheated Rotors
FIG. X3.2 Example of an ODC Rotor With Provision for Heating
D 2084 X3.5 The precision and bias of ODC tests run with the alternative heated biconical disk have not been statistically determined. The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org).